Ultrafast and Distinct Spin Dynamics in Magnetic Alloys
I. Radu*,†,**,††, C. Stamm†,‡‡, A. Eschenlohr†,§§, F. Radu‡, R. Abrudan§, K. Vahaplar*, T. Kachel†, N. Pontius†, R. Mitzner†, K. Holldack†, A. F€ohlisch†,
T. A. Ostler¶, J. H. Mentink*, R. F. L. Evans¶, R. W. Chantrell¶, A. Tsukamoto||, A. Itoh||,A. Kirilyuk*, A. V. Kimel*and Th. Rasing*
*Radboud University, Institute for Molecules and Materials Heyendaalseweg 135, 6525 AJ Nijmegen, The Netherlands
†Institut f€ur Methoden und Instrumentierung der Forschung mit Synchrotronstrahlung
Helmholtz-Zentrum Berlin f€ur Materialien und Energie GmbH Albert-Einstein-Straße 15, 12489 Berlin, Germany
‡Institut f€ur Komplexe Magnetische Materialien
Helmholtz-Zentrum Berlin f€ur Materialien und Energie GmbH Albert-Einstein-Straße 15, 12489 Berlin, Germany
§Institut f€ur Experimentalphysik/Festk€orperphysik Ruhr-Universit€at Bochum, 44780 Bochum, Germany
¶Department of Physics, University of York Heslington, York YO10 5DD, United Kingdom
||College of Science and Technology
Nihon University, 7-24-1 Funabashi, Chiba, Japan **firstname.lastname@example.org
Received 23 May 2015 Accepted 26 May 2015 Published 20 August 2015
Controlling magnetic order on ultrashort timescales is crucial for engineering the next-generation magnetic devices that combine ultrafast data processing with ultrahigh-density data storage. An appealing scenario in this context is the use of femtosecond (fs) laser pulses as an ultrafast, external stimulus to fully set the orientation and the magnetization magnitude of a spin ensemble.
††Currently with the Institute for Optics and Atomic Physics Technical University Berlin, Germany.
‡‡Currently with the Department of Material Science, ETH Zürich Schafmattstr. 30, 8093 Zürich, Switzerland.
§§Currently with Fakultät für Physik, Universität Duisburg-Essen Lotharstr. 1, 47057 Duisburg, Germany.
This is an open access article published by World Scienti¯c Publishing and distributed under the terms of the Creative Commons Attribution (CC BY) 4.0 License, which permits use, distribution and reproduction in any medium, provided the original author(s) and source are credited.
Vol. 5, No. 3 (2015) 1550004 (10 pages)
© The Authors
Achieving such control on ultrashort timescales, e.g., comparable to the excitation event itself, remains however a challenge due to the lack of understanding the dynamical behavior of the key parameters governing magnetism: The elemental magnetic moments and the exchange interaction. Here, we investigate the fs laser-induced spin dynamics in a variety of multi-com-ponent alloys and reveal a dissimilar dynamics of the constituent magnetic moments on ultrashort timescales. Moreover, we show that such distinct dynamics is a general phenomenon that can be exploited to engineer new magnetic media with tailor-made, optimized dynamic properties. Using phenomenological considerations, atomistic modeling and time-resolved X-ray magnetic circular dichroism (XMCD), we demonstrate demagnetization of the constituent sub-lattices on signi¯-cantly di®erent timescales that depend on their magnetic moments and the sign of the exchange interaction. These results can be used as a \recipe" for manipulation and control of magnetization dynamics in a large class of magnetic materials.
Keywords: Ultrafast spin dynamics; element-speci¯c magnetization; atomistic spin simulations.
Femtosecond (fs) laser-induced controlling of fer-romagnetic order1 has intrigued researchers since the pioneering work of Beaurepaire et al.,2 who found that fs optical excitation of ferromagnetic Ni can demagnetize the sample on a sub-picosecond time-scale. This demagnetization event was much faster than one might expect supposing that the demagnetization process is de¯ned by the charac-teristic time of the spin-lattice relaxation in the ground state. Later, it was demonstrated that cir-cularly polarized laser pulses could act as equally short and relatively strong e®ective magnetic ¯eld pulses,3 even leading to fs laser-induced switching of the magnetization.4 These intriguing observa-tions have triggered intense experimental and the-oretical e®orts to understand the fundamental processes underpinning such ultrafast laser-induced dynamics.1 Although a few models of laser-induced demagnetization of simple ferromagnets such as Ni, Fe, Co and Gd have been suggested,5–7 the physics of ultrafast magnetic phenomena in systems with two or more magnetic sublattices8–13 still chal-lenges our understanding. Yet many magnetization dynamics studies were performed with magnetic compounds containing at least two magnetic ele-ments, like the well-known Permalloy,14–16 ortho-ferrites,3 manganites17 and yttrium–iron–garnets.18 In the conventional macrospin approximation,1 the constituent magnetic sublattices of an alloy are represented by a single macrospin [see Fig. 1(a)], which is used to describe their static and dynamic properties. This implies that two exchange-coupled magnetic sublattices are dynamically indistin-guishable and thus would lose their magnetization
on the very same time-scale upon ultrafast (fs) laser excitation. However, recent experiments using fs X-ray magnetic circular dichroism (XMCD) have revealed distinctly di®erent magnetization dynamics of the constituent magnetic moments in a Gd(FeCo) alloy excited by a fs optical pulse.10 Moreover, it was subsequently shown19 that these distinct dynamics in combination with the ex-change interaction between the sublattices, can lead to a deterministic switching of this ferrimag-netic Gd(FeCo) by an ultrafast heat pulse alone.20 These results lead to the intriguing question of whether such element-speci¯c spin dynamics is a general phenomenon or something strictly related
Fig. 1. Schematic illustration of the conventional (a) and of the ultrafast and distinct (b) spin dynamics. In the conventional picture (a) the dynamics of spin systems consisting of several magnetic elements is treated in the macrospin approximation where all the constituent elements are treated as a single mac-rospin. Within the ultrafast and distinct spin dynamics picture (b), one accounts for the dynamics of each magnetic constituent of a multi-component magnetic alloy separately, their dynamics being governed by the magnitude of their magnetic moment (the arrows in the ¯gure) and by their mutual exchange inter-action (the springs in the ¯gure).
to a narrow class of GdFe-like ferrimagnetic materials?
Here, we investigate the dynamics of multi-sub-lattice magnetic materials with both ferromagnetic and antiferromagnetic coupling between their sub-lattices. Using phenomenological modeling and atomistic spin simulations, we show that their de-magnetization dynamics is distinct and element-speci¯c. These simulations are fully supported by element-speci¯c fs time-resolved XMCD experi-ments on various NiFe and rare earth-transition metal (RE-TM) alloys, which provide evidence for a demagnetization time that scales with the elemental magnetic moment and varies with the sign of the exchange interaction. As such, one can tune the speed of magnetization processes in multi-sublattice alloys by properly choosing the magnitude of the constituent magnetic moments and the sign of the exchange interaction that couples them. These results may lead to new design principles of mag-netic media for fast and energy-e±cient magmag-netic data manipulation and storage.12,13,23
2. Phenomenological Model of Ultrafast Magnetization
Dynamics in Ferromagnetic Alloys
To gain a qualitative understanding of the ultrafast demagnetization dynamics in ferromagnetically or-dered two-sublattice magnets, we employ a macro-scopic theory developed originally by Baryakhtar21 for the description of the dynamics and relaxation of the macroscopic (sublattice) magnetization of fer-romagnets and antiferfer-romagnets. It was recently shown that this approach can qualitatively describe the spatially averaged and dominantly longitudinal dynamics obtained from atomistic spin dynamics simulations.8 Clearly, the Baryakhtar theory is not restricted to longitudinal dynamics, and it has re-cently been demonstrated22 for antiferromagnetic coupling in the exchange approximation, that in addition to the purely longitudinal solutions, the theory exhibits a second class of solutions, which for speci¯c conditions allows for the appearance of transverse time evolution with the same timescale as the longitudinal exchange relaxation. For the pres-ent work, we are interested in a di®erpres-ent regime, where both the relativistic relaxation as well as the exchange relaxation play an important role (regime 3 according to Ref.8), and we will restrict ourselves
to the class of longitudinal solutions only. This approach is supported by atomistic simulations,23 which show that even when the system exhibits a small canting before laser excitation, the fast initial relaxation directly after excitation, i.e., the ultrafast demagnetization, is dominantly longitudinal. Fur-thermore, all experiments that operate at macro-scopic length scales, including the X-ray experiments we describe below, demonstrate a longitudinal evolution of the (sublattice) magnetization on the sub-picosecond timescale. Hence on macroscopic length scales, the longitudinal time-evolution seems to be the relevant one. Under these conditions, the equations of motion are:
_S1¼ 1H1þ eðH1 H2Þ; ð1aÞ _S2¼ 2H2þ eðH2 H1Þ; ð1bÞ where Si denotes the macroscopic spin angular mo-mentum of sublattice i¼ 1; 2, and Hi ¼ W=Siis the e®ective magnetic ¯eld for sublattice i, which is derived from the magnetic (Landau) free energy W. i are the relativistic relaxation parameters de-scribing the transfer of angular momentum with the environment, while e describes the exchange relaxation responsible for transfer of angular mo-mentum between the sublattices. Previous work8 considered both i;e and the free energy W as phe-nomenological parameters. As a next step, to assess the in°uence of the concentration, we derive the macroscopic free energy from a microscopic Heisenberg model, which is also the basis for atom-istic spin dynamics simulations. Hence, similar to the latter, we explicitly assume that the longitudinal time-evolution on the macroscopic scale originates from spatial averaging over the transverse dynamics of the atomistic spins. Using the methods described in e.g., Refs. 24–26, we obtain in the mean ¯eld approximation for classical spins and for small Si values: W ¼ 2N1 11S 2 1þ2N1 22S 2 2N2Np 1N2J12S1S2; ð2aÞ 1i ¼ 3 2 1 kBT 2ziiJii: ð2bÞ For a binary alloy, we can use N1¼ ð1 xÞN, N2¼ xN, Np¼ xð1 xÞzN, z11¼ z21¼ ð1 xÞz, z22¼ z12¼ xz, where x is the concentration of sub-lattice 2, z the average number of nearest neighbors
in the alloy, and N the total number of spins per unit volume. In addition, i indicates the magnitude of the spin angular momentum in sublattice i and Jij are exchange parameters between spins in sublattice i and j that we take for nearest neighbors only. Further, kBT is the energy of the temperature °uc-tuations experienced by the spins, which we assume to be solely determined by the electron temperature. In principle, it is possible to extract the relaxation parameters from microscopic theory in a similar way as ¯rst-principle calculations of the trans-verse Gilbert relaxation parameter.27,28 This will generally yield parameters that depend on the temperature, the exchange interactions and the concentration. Below, we will consider the relaxa-tion parametersi;e as purely phenomenological, in order to gain qualitative understanding in the limits of small and large concentration.
To understand qualitatively how the demagneti-zation time changes by going from the pure element to the alloy, we consider ¯rst the limiting case of small x. In this limit, we simplify the theory using eðxÞ i for x 1 and the transfer of angular momentum between the sublattices will in general be a small e®ect. Furthermore, this transfer is gen-erally less e®ective for ferromagnetic coupling than for antiferromagnetic coupling, since the terms in H1 H2 partly cancel each other. Therefore, we can write the demagnetization rate after a (fs laser-induced) step-like change of the electron tempera-ture as _S1¼ 1H1. Using Eqs. (2a) and (2b) with S1jt¼0¼ N11ðxÞ we ¯nd:
_S1ðxÞ ¼ 1ðxÞ½3kBT ð1 xÞzJ11 xzJ12=1ðxÞ: ð3Þ As in the pure material, we ¯nd a demagnetization time that depends on the magnetic moment, and hence the Ni and Fe sublattices generally have dis-tinct dynamics after laser excitation due to the dif-ference in their magnetic moments. In addition, the concentration determines the sublattice magnetic moments and exchange coupling strength, which can be di®erent from the pure material. This in turn leads to a change in demagnetization times com-pared to the pure material. Applying this to the NiFe alloy at small Fe concentration, we have JNiNi < JNiFe.29Since alsoNið0Þ < NiðxÞ30(see also Supplementary Sec. 6), we anticipate the de-magnetization time of Ni increases upon moderate doping with Fe.
Next, we investigate the limit of large con-centration (x 0:5). As before, the relativistic contributions generally yield distinct dynamics, however the transfer of angular momentum between the sublattices may not be negligible anymore. For example, at high-temperature (kBT Jij) we have H1 H2 3kBT ð11 12 Þ ¼ þ3kBT ð1 2Þ= 12. The sign of this term depends on the di®erence 1 2, which suggests an additional acceleration (deceleration) of sublattice 1 (2) when 1< 2. Unfortunately, it is not straightforward to apply this analysis to the case of NiFe, since for large concentration the system is in the Invar region. In this regime, the Ni sublattice remains almost col-linear with the average magnetization, but the Fe sublattice is essentially frustrated and noncollinear even at very low temperature. This frustration is caused by long-range oscillating exchange interac-tions31 and due to local environment e®ects that yield a huge dispersion of the nearest-neighbor ex-change parameters,32 which results in a decrease of the Curie temperature despite the fact that the magnitude of the exchange interactions increases.33 Although the assessment of such frustrated magne-tism goes beyond the nearest-neighbor Heisenberg model employed here, we anticipate that an essen-tially noncollinear Fe environment can allow for an e±cient transfer of angular momentum between the sublattices (large parameter eÞ, which in the high-temperature limit yields an acceleration of the demagnetization of Ni, sinceNi< Fe. This accel-eration counteracts the decelaccel-eration due to the in-crease of Ni, which in the Invar regime is almost twice as large as in pure Ni. Hence, the exchange relaxation in the Invar regime can make the dy-namics of Ni and Fe more distinct than anticipated solely from the di®erence of the magnetic moments, which is indeed the trend observed in the atomistic and experimental results shown below.
3. Atomistic Spin Simulations of Ultrafast Demagnetization
Following the model predictions above, we have performed atomistic simulations of the response of 106 ferromagnetically exchange-coupled NiFe as well as antiferromagnetically coupled GdFe spins to an ultrashort 60 fs heat pulse, as explained in the Supplementary Information. The dynamics of each magnetic sublattice were obtained by solving a
system of coupled stochastic Landau–Lifshitz– Gilbert equations for individual atomic moments, which describe the transient dynamics of the system upon excitation with a fs laser pulse.34 For multi-component magnetic alloys one derives34,35 a characteristic longitudinal relaxation timea (i.e., demagnetization time) for each constituent compo-nent which scales with:
2iikBT ; ð4Þ wherei is the moment associated with site i; i is the coupling constant to the thermal bath,i is the gyromagnetic ratio at site i, kB is Boltzmann's constant and T is the temperature of the bath. Consequently, if an alloy consists of two sublattices and 16¼2, a rapid heating of the system to high temperatures will lead to di®erent demagnetization dynamics of the two sublattices, despite the strong exchange interaction that couples them. The e®ect ofiandion the demagnetization time is discussed in Supplementary Sec. 7.
We have simulated both ferromagnetically pled NiFe alloys as well antiferromagnetically cou-pled GdFe (ferrimagnetic) systems. Following Ref.34, we coupled the spin system to the electron temperature that is calculated using the two-temperature model,36 which describes the transient variation of the electron and phonon temperatures upon femtosecond laser excitation. The strength of the thermal °uctuations then scales with this time-varying temperature. For simplicity, the model assumes the same coupling constants for the di®er-ent sublattices (i¼ 0:01), and the magnetic moments were derived from XMCD measurements (see Supplementary Information). The NiFe ex-change interactions were determined from the measured Curie temperature of the NiFe alloy samples as reported in Ref.37. For instance, in the case of Ni50Fe50, this yields a total exchange per spin of 260 meV. The results of the Ni50Fe50 simulations are displayed in Fig. 2(a), showing clearly a faster demagnetization for Ni than for Fe. This conclusion holds for the full stoichiometry range of the NiFe alloys, as detailed in the Supplementary Sec.6.
To simulate the antiferromagnetically coupled GdFe system, we used the exchange constants obtained by ¯tting the temperature-dependent
XMCD data measured for the Fe and Gd sub-lattices.35Taking into account the number and type of neighbors, the total e®ective Fe–Gd exchange is 30 meV. The results of the GdFe simulations are displayed in Fig. 2(b), showing a dissimilar demag-netization dynamics of Fe and Gd with Fe being much faster than Gd.
Hence, distinct timescales for the demagnetiza-tion of magnetic sublattices have been computed for both ferromagnetic and antiferromagnetic coupling between the sublattices. Thus, this appears to be a general phenomenon for multi-sublattice magnets.
Fig. 2. Computed transient dynamics of the constituent magnetic moments in FeNi and GdFe alloys using the atomistic spin model. The response of the longitudinal component of the magnetization of Ni and Fe in Ni50Fe50alloy (a) and of Fe and Gd in Gd24Fe76alloy (b) to a 60 fs laser pulse. The dashed lines in both panels display the transient electronic temperature used in the simulation. The starting temperature for the simulation is 300 K. Note that in panel (b) the Fe and Gd curves are merging together around 1.8 ps (see Supplementary Information Sec.3).
aThe longitudinal relaxation time denotes here the decay of the z component of the volume-averaged magnetic moment (whose
length is locally conserved).
4. Ultrafast Dynamics of the Elemental Magnetic Moments from
Time-Resolved XMCD Experiments
To compare these theoretical predictions and simulations with experiments, we measured the transient demagnetization dynamics of the mag-netic sublattices in NiFe and GdFe alloysbas well as their respective pure elements, employing the ele-ment-speci¯c XMCD technique in transmission at the femto-slicing facility38,39 of the Helmholtz– Zentrum Berlin. In addition, we have also investi-gated a ferrimagnetic DyCo5 (i.e., Dy16:7Co83:3) alloy40that shows the largest di®erence between the magnitudes of the constituent magnetic moments (see Supplementary Fig. 3). The experiments were performed in a stroboscopic pump-and-probe mode, where the metallic samples were excited with 60 fs laser pulses of 1.55 eV photon energy. Subsequent laser-induced magnetization dynamics were probed by measuring the XMCD changes in transmission with circularly polarized 100 fs X-ray pulses39tuned at the L3 edges of Ni (853 eV), Fe (707 eV), Co (778 eV) and at the M5 edges of Gd (1189 eV) and Dy (1292 eV). At these energies, we probe the dy-namics of the 3d magnetic moment of Ni, Fe, Co and the 4f moment of Gd and Dy, respectively. We point out that at these absorption edges, there is a nonambiguous relationship between the measured XMCD signal and the elemental magnetic moments41 that remains valid even in the high nonequilibrium regime after laser excitation.42 The XMCD measurements were performed on Fe, Ni, Ni50Fe50, Ni80Fe20, Dy16:7Co83:3 and Gd25Fe66Co9 samples at 300 K except for DyCo5, which were done at 100 K (under laser exposure the e®ective sample temperature of DyCo5 rose well above its compensation temperature of 120 K due to a per-manent heating e®ect, as deduced from the polarity of the XMCD signal and the elemental hysteresis). For Gd(FeCo), the magnetization compensation temperature was 250 K. The typical absorbed laser °uence was 6.8 mJ/cm2 for NiFe alloys, 10.1 mJ/cm2
for DyCo5 while for Gd(FeCo) it was 4.5 mJ/cm2. The Fe, Ni and NiFe ¯lms exhibit an in-plane magnetization orientation, while Gd(FeCo) and DyCo5 have an out-of-plane mag-netic anisotropy. The samples are poly-crystalline except for Gd(FeCo) which is amorphous.
The results of the element-speci¯c laser-induced demagnetization of ferromagnetic Ni50Fe50 are shown in Fig. 3(a). Upon fs laser excitation, the alloy demagnetizes to about 50% at both the Fe and Ni edges. Although a similar degree of demagneti-zation is achieved for both elements, their transient demagnetization behavior is considerably di®erent: While Fe is demagnetized within 800 fs, it takes only 300 fs for Ni to demagnetize to the same extent as Fe, in qualitative agreement with the
Fig. 3. Element-speci¯c demagnetization dynamics of the constituent magnetic moments in FeNi and GdFe alloys measured by time-resolved XMCD with fs time-resolution. El-ement-speci¯c demagnetization measured in (a) ferromagnetic Ni50Fe50at the Fe L3and Ni L3edges and (b) in ferrimagnetic
Gd25Fe66Co9alloy at the Fe L3and Gd M5edges. The solid lines
are ¯ts according to a bi-exponential ¯t function (see Eq. (5)). The Gaussian pro¯les depict the time resolution of the XMCD measurements of 130 fs.
bThe GdFe sample contained a small percentage (9%) of Co to control the magnetic anisotropy— for more details, see
Supple-mentary Information Sec. 1.
predictions from Fig. 2(a). Although less pro-nounced, we measure similar distinct demagnetiza-tion dynamics of the Fe and Ni moments in a Ni80Fe20sample with again Fe being slower than Ni (see Supplementary Fig. 7).
Essentially, a similar decoupled demagnetization behavior of the constituent, but antiferromagneti-cally coupled, magnetic moments is encountered for the ferrimagnetic Gd(FeCo) alloy, as shown in Fig. 3(b). In this case, the demagnetization of Fe takes 400 fs while Gd demagnetizes within 1.2 ps. Due to the lower TC of 550 K (see Ref.35), here we totally quench the magnetic order at both Fe and Gd edges i.e., achieve a demagneti-zation degree of 100%. This dynamic decoupling of Fe and Gd is however also encountered for much lower demagnetization degrees down to 40% (see Supplementary Fig. 8).
For the ferrimagnetic alloy DyCo5, according to Eq. (4) and given the di®erent values of the con-stituent Co ( 1.52 B) and Dy ( 8.91 B) magnetic moments (see Supplementary Fig. 3), we expect a large di®erence between their dynamics. Indeed, as shown in Supplementary Fig. 9, Co demagnetizes down to 50% within 350 fs while it takes several ps for Dy to reach the same demagnetization level.
To extract the time constants of the measured demagnetization transients, we have used the fol-lowing bi-exponential ¯t function:
fðtÞ ¼ gðtÞ A B exp t D þ C exp t R ; ð5Þ where D and R are the demagnetization and relaxation time constants, g(t) is the Gaussian function describing the time resolution of the ex-periment, B and C are the exponential amplitudes and A is the value of the transient signal at negative delays. The demagnetization time constants obtained from the ¯ts are listed in Table 1 of Sup-plementary Information and plotted in Fig. 4(a). For comparison, we also show the demagnetization time constants of the elemental Fe, Ni, Co and Gd samples. The demagnetization of pure Co and Gd are taken from Refs. 5 and 43, respectively. For demagnetization of pure Ni, please see also Ref. 44. We note that these demagnetization time constants are extracted from demagnetization transients (both
the alloys and their elemental counterparts) that exhibit similar demagnetization degreesM=M0 of around 50%, and thus we can treat and compare these demagnetization times on equal footing. In Fig. 4(b) we show the deduced demagnetization constants versus magnetic moment for all measured samples. One observes a clear scaling behavior be-tween the demagnetization time and the magnitude of the magnetic moment. A quantitative estimate for the variation of the demagnetization time per magnetic moment unit is obtained by ¯tting the
Fig. 4. The experimental demagnetization time constants measured for single Ni, Fe, Co and Gd elements and their alloys. In panel (a), we show the overview of the demagnetization time constants of the elemental magnetic moments in the Ni80Fe20, Ni50Fe50, DyCo5and Gd25Fe66Co9alloys and of the pure Fe, Ni,
Co and Gd samples. The solid lines are guides to the eye. De-magnetization time constants of pure Co and Gd are taken from Refs.5and43, respectively, while the demagnetization of Co in CoPd alloy is taken from Ref.45. The gray regions emphasize the dissimilar demagnetization time constants of the elements in the same alloy. Panel (b) shows the dependence of the demag-netization time constants from panel (a) on the magnitude of the elemental magnetic moments for pure elements and their alloys. The solid line is a linear ¯t to the data.
data using a linear ¯t function [the solid line in Fig.4 (b)], which gives us a value of90 20 fs/B.
Another important piece of information provided by these data is the dependence of the demagneti-zation time on the magnetic ordering type of the samples. This is shown in Fig. 5 where the demag-netization time constants of Fe and Co are plotted for pure samples, ferromagnetic FeNi and CoPd and ferrimagnetic (i.e., antiferromagnetic coupling) Gd (FeCo) and DyCo alloys. For a ferromagnetic type of coupling, both the Fe and Co moments demag-netize slower than the pure material while the op-posite is observed in the antiferromagnetically coupled GdFe and DyCo. Please note that the very same behavior is encountered when normalizing the elemental demagnetization times to the corre-sponding magnetic moment magnitudes.
There are three major e®ects that can be observed in the overview of the demagnetization time constants shown in Figs. 4 and 5: (i) The distinctly di®erent demagnetization times of the elemental magnetic moments in the ferromagnetic NiFe and ferrimag-netic Gd(FeCo) and DyCo5 alloys [the highlighted regions in Fig.4(a)], (ii) the demagnetization times scale approximately with the magnitude of the ele-mental magnetic moment [see Fig.4(b)] for the pure samples of Ni, Fe, Co and Gd as well as for their alloys and (iii) the demagnetization time of a speci¯c element (e.g., Fe or Co) changes with the exchange
interaction type of the host alloy i.e., it is longer in ferromagnetic FeNi and shorter in antiferro-magnetically coupled Gd(FeCo) and DyCo5 com-pared to their pure Fe and Co counterparts (see Fig.5).
Both the XMCD data and the simulations show that, despite the strong ferromagnetic exchange coupling between the Ni and Fe sublattices in NiFe, they apparently lose their net magnetization in a very dissimilar manner. The same situation is also observed in ferrimagnetic Gd(FeCo) and DyCo5, where two antiferromagnetically coupled Gd and Fe or Dy and Co sublattices demagnetize on substan-tially di®erent time-scales. Thus, we observe the same transient decoupling of the exchange-coupled magnetic moments in two material systems that are strikingly di®erent, i.e., ferromagnetic versus anti-ferromagnetic coupling, itinerant versus localized type of magnetic ordering and in-plane versus out-of-plane magnetic anisotropy. Consequently this distinct dynamics seems to be a general property of multi-elemental magnetic compounds that are driven nonadiabatically to a highly nonequilibrium state by fs laser excitation. Moreover, in agreement with Eqs. (3) and (4), the observed characteristic demagnetization times scale with the magnetic moment of the sublattices i.e., the larger the mag-netic moment the slower the demagnetization pro-cess [see Fig. 4(b)]. For the materials investigated here, we obtain a characteristic change of the demagnetization time per magnetic moment of 90 20 fs/B. Consequently, although in NiFe, Fe demagnetizes slower than Ni, in Gd(FeCo) the de-magnetization of the Fe-sublattice is much faster than the demagnetization of Gd. This distinct dy-namics is even more pronounced in DyCo5given the large di®erence (a factor of 6) between the Dy and Co magnetic moments.
Furthermore, the antiferromagnetic coupling in Gd(FeCo) and DyCo5yields faster demagnetization of both sublattices when compared to their pure elements. The ferromagnetic coupling in Ni50Fe50, on the other hand, yields faster demagnetization of Ni and slower demagnetization of Fe, despite the fact that the magnetic moment of Ni increases (see Supplementary Fig. 3 for variation of the magnetic moment with the sample stoichiometry). In Ni80Fe20, the exchange coupling between the sublattices is not e®ective enough (see Table 2 in Supplementary Information) to compensate for the increased magnetic moment, yielding an increase of Fig. 5. The dependence of the demagnetization times for Fe
and Co on the magnetic ordering type of the host alloys. Comparison of the demagnetization time constants measured for Fe and Co in ferromagnetic FeNi and CoPd, ferrimagnetic GdFeCo and DyCo as well as for pure elements. The demag-netization time constants for pure Co and Co in CoPd are taken from Refs.5and45, respectively.
the demagnetization time of Ni compared to the pure case.
Overall, these results show that is possible to control the dynamics of the constituent sublattices in magnetic alloys by changing the magnitude of the magnetic moment of the constituent elements, the sign and strength of the exchange interaction or a combination thereof. Moreover, knowing the key parameters that govern the ultrafast magneti-zation dynamics in alloys, we can extend this \recipe" and hypothesize that magnetization dy-namics can be engineered the very same way in arti¯cial magnetic structures mimicking the intrinsic properties of alloys, as for instance in synthetic ferrimagnets.46
Before concluding the paper, we would like to discuss the relevance of the recent transversal mag-neto-optical Kerr e®ect (TMOKE) results by Mathias et al.15 in the context of our study. These authors used time-resolved magneto-optics in re-°ection to investigate the laser-induced demagneti-zation of pure Fe, Ni and of a permalloy (Ni80Fe20) sample. By tuning the probing VUV photon energy at the M3;2 (3p–3d transitions) resonances of Ni ( 67 eV) and Fe ( 54 eV) they report that Fe demagnetizes quicker than Ni in pure samples while in Permalloy both elements exhibit the same demagnetization time (about 240 fs) and a time lag in the onset of their respective transient dynamics. There are two major di®erences between our work and the study of Ref. 15: (i) Their measurements were performed in re°ection geometry and (ii) magnetization dynamics has been probed at the M3;2 elemental edges in the VUV spectral range. Regarding point (i), magneto-optical X-ray mea-surements performed in re°ection do not provide a direct, quantitative measure of the elemental mag-netic moment, which is at variance compared to their transmission counterparts.41 This is because the magneto-optical signal measured in re°ection consists of an admixture of dispersive and absorptive parts of the dielectric function, and as such the use of the sum rulescto determine the magnetic moment is inapplicable. Second, in the VUV spectral range the energies corresponding to the spin-orbit and the exchange interactions are of comparable magnitude, which leads to a strong distortion of the 3p electronic states of Ni and Fe (the M3and M2absorption edges
are essentially overlapped) and consequently, one cannot apply the sum rules to obtain the magnitude of the magnetic moment (see e.g., Ref. 47). This is valid for both re°ection and absorption measure-ments. Moreover, in the VUV range, the close en-ergetic proximity of Fe and Ni absorption edges results in an overlap of their respective magnetic signals; this renders, for such alloys, the interpreta-tion of the magnetizainterpreta-tion data in terms of pure ele-mental response more di±cult and ambiguous. Also, the time-resolved TMOKE measured in the VUV range might be susceptible to magneto-optical arti-facts, as has been recently pointed out by Vodungbo et al.48 Thus, the TMOKE signal might contain nonmagnetic contributions that complicate the in-terpretation of the data as being only of magnetic origin.
In short, due to their measurement speci¯city, the results of Mathias et al.15 do not provide informa-tion about the dynamics of the elemental magnetic moment in their samples. This is at variance with our present work performed in the soft X-ray spec-tral range, which allows the accurate application of the magneto-optical sum rules and thus providing a nonambiguous relationship between the measured signal and the magnetic moment. As such, there is no common basis for comparing our results with those reported in Ref.15 as this work is essentially measuring di®erent observables.
To conclude, our atomistic spin modeling and phe-nomenological theory, supported by element-speci¯c fs XMCD experiments, demonstrate the possibility of tuning the dynamics of multi-sublattice ferro-magnets and ferriferro-magnets by their composition, which determines their magnetic moments and the strength of the exchange interaction. This can lead to distinctly di®erent demagnetization times even for the same element in di®erent alloys. In particu-lar, we have shown that for antiferromagnetic coupling, exchange relaxation accelerates the de-magnetization of both sublattices, while with ferro-magnetic coupling, the dynamics of one sublattice is accelerated while the other is slowed down. Fur-thermore, we have shown that, by tuning the com-position we can control the distinctiveness of the
cThe magneto-optical sum rules relate the absorption cross-section with the ground-state expectation values of the spinhSzi and
orbitalhLzi moments. SPIN Downloaded from www.worldscientific.com by 188.8.131.52 on 08/20/15. For personal use only.
sublattice dynamics. This allows designing new magnetic materials, for example using exchange coupled multilayers, which combine desirable prop-erties for future recording media.12,13,23
Funding from the European Community's Seventh Framework Program (FP7/2007–2013) Grants No. NMP3-SL-2008-214469 (UltraMagnetron), No. 214810 (FANTOMAS) and No. 281043 (FEMTOSPIN) and ERC Grant No. 257280 (Femtomagnetism) as well as Grant No. 226716 and ERC-2013-AdG339813-EXCHANGE, the German Federal Ministry of Education and Research (BMBF) Grant No. 05K10PG2 (FEMTOSPEX), the Foundation for Fundamental Research on Matter (FOM) and the Netherlands Organization for Scienti¯c Research (NWO) is gratefully acknowledged.
1. A. Kirilyuk, A. V. Kimel and Th. Rasing, Rev. Mod. Phys. 82, 2731 (2010).
2. E. Beaurepaire, J.-C. Merle, A. Daunois and J.-Y. Bigot, Phys. Rev. Lett. 76, 4250 (1996).
3. A. V. Kimel et al., Nature (London) 429, 850 (2004). 4. C. D. Stanciu et al., Phys. Rev. Lett. 99, 047601
5. B. Koopmans et al., Nature Mater. 9, 259 (2010). 6. M. Battiato, K. Carva and P. M. Oppeneer, Phys.
Rev. Lett. 105, 027203 (2010).
7. J.-Y. Bigot, M. Vomir and E. Beaurepaire, Nature Phys. 5, 515 (2009).
8. J. Mentink et al., Phys. Rev. Lett. 108, 057202 (2012).
9. S. Wienholdt et al., Phys. Rev. B. 88, 020406 (2013). 10. I. Radu et al., Nature (London) 472, 205 (2011). 11. N. Bergeard et al., Nature Commun. 5, doi: 10.1038/
12. S. Mangin et al., Nature Mater. 13, 286 (2014). 13. C. H. Lambert et al., Science 345, 1337 (2014). 14. C. La-O-Vorakiat et al., Phys. Rev. Lett. 103,
15. S. Mathias et al., P. Natl Acad. Sci. USA 109, 4792 (2012).
16. I. Radu et al., Phys. Rev. Lett. 102, 117201 (2009). 17. T. Lottermoser et al., Nature 430, 541 (2004). 18. S. O. Demokritov et al., Nature 443, 430 (2006). 19. T. Ostler et al., Nature Commun. 3, 666 (2012). 20. J. Barker et al., Scienti¯c Reports 3, 03262 (2013). 21. V. G. Baryakhtar Sov. Phys. JETP 60, 863 (1984). 22. V. G. Baryakhtar, V. I. Butrim and B. A. Ivanov,
JETP Lett. 98, 289 (2013).
23. R. Evans et al., Appl. Phys. Lett. 104, 082410 (2014).
24. H. Falk, Am. J. Phys. 38, 858 (1970).
25. O. F. Abubrig et al., Physica A 296, 437 (2001). 26. J. W. Negele and H. Orland, Quantum
Many-Particle Systems (Westview Press, Boulder USA, 1988).
27. H. Ebert et al., Phys. Rev. Lett. 107, 066603 (2011). 28. A. A. Starikov et al., Phys. Rev. Lett. 105, 236601
29. P. Yu et al., Phys. Rev. B 77, 054431 (2008). 30. B. Glaubitz et al., J. Phys.: Condens. Matter 23,
31. M. van Schilfgaarde et al., Nature 400, 46 (1999). 32. A. V. Ruban et al., Phys. Rev. B 71, 054402 (2005). 33. J. Kudrnovský et al., Phys. Rev. B 77, 224422
34. N. Kazantseva et al., Europhys. Lett. 81, 27004 (2008).
35. T. Ostler et al., Phys. Rev. B. 84, 024407 (2011). 36. S. I. Anisimov, B. L. Kapeliovich and T. L.
Perel-man, Sov. Phys. JETP 39, 375 (1974).
37. E. H. Wasserman, in Ferromagnetic Materials, Vol. 5 (Elsevier, Amsterdam , The Netherlands, 1990). 38. C. Stamm et al., Nature Mater. 6, 740 (2007). 39. S. Khan et al., Phys. Rev. Lett. 97, 074801 (2006). 40. F. Radu, R. Abrudan, I. Radu, D. Schmitz and H.
Zabel, Nature Commun. 3, 715 (2012).
41. C. T. Chen et al., Phys. Rev. Lett. 75, 152 (1995). 42. K. Carva et al., Europhys. Lett. 86, 57002 (2009). 43. M. Wietstruk et al., Phys. Rev. Lett. 106, 127401
44. C. Stamm et al., Phys. Rev. B 81, 104425 (2010). 45. C. Boeglin et al., Nature 465, 458 (2010).
46. R. Evans, T. Ostler, R. Chantrell, I. Radu and Th. Rasing, Appl. Phys. Lett. 104, 082410 (2014). 47. D. Zhao et al., J. Appl. Phys. 84, 2858 (1998). 48. B. Vodungbo et al., Phys. Rev. X 3, 038001 (2013). SPIN Downloaded from www.worldscientific.com by 184.108.40.206 on 08/20/15. For personal use only.